DOI: 10.17188/1308806
title: Materials Data on Li12Mn5V3(PO4)12 by Materials Project

description: Li12V3Mn5(PO4)12 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.52 Å. In the second Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.64 Å. In the third Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.03 Å. In the fourth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.04 Å. In the fifth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.59 Å. In the sixth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.53 Å. In the seventh Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.55 Å. In the eighth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.65 Å. In the ninth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.02 Å. In the tenth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.04 Å. In the eleventh Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.59 Å. In the twelfth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.51 Å. There are three inequivalent V+4.67+ sites. In the first V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.91–2.21 Å. In the second V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.95–2.09 Å. In the third V+4.67+ site, V+4.67+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.91–2.12 Å. There are five inequivalent Mn2+ sites. In the first Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.92–2.41 Å. In the second Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.90–2.16 Å. In the third Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.90–2.16 Å. In the fourth Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.92–2.38 Å. In the fifth Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.92–2.41 Å. There are twelve inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 28–43°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 12–45°. There are a spread of P–O bond distances ranging from 1.52–1.58 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 17–46°. There are a spread of P–O bond distances ranging from 1.51–1.58 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 13–48°. There are a spread of P–O bond distances ranging from 1.51–1.57 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 23–47°. There are a spread of P–O bond distances ranging from 1.54–1.57 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 30–44°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 31–43°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 17–46°. There are a spread of P–O bond distances ranging from 1.53–1.58 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 18–45°. There are a spread of P–O bond distances ranging from 1.51–1.58 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 16–48°. There are a spread of P–O bond distances ranging from 1.51–1.57 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 23–46°. There are a spread of P–O bond distances ranging from 1.54–1.58 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 30–42°. There is three shorter (1.54 Å) and one longer (1.56 Å) P–O bond length. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the second O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the third O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.67+, and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.67+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the seventh O2- site, O2- is bonded in a linear geometry to one V+4.67+ and one P5+ atom. In the eighth O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form distorted edge-sharing OLi2MnP tetrahedra. In the ninth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+4.67+, and one P5+ atom. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+4.67+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted linear geometry to one V+4.67+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form distorted OLi2MnP tetrahedra that share a cornercorner with one OLi2VP tetrahedra and an edgeedge with one OLi2MnP tetrahedra. In the seventeenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+4.67+, and one P5+ atom. In the nineteenth O2- site, O2- is bonded to two Li1+, one V+4.67+, and one P5+ atom to form distorted corner-sharing OLi2VP tetrahedra. In the twentieth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+4.67+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.67+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form distorted OLi2MnP tetrahedra that share a cornercorner with one OLi2VP tetrahedra and an edgeedge with one OLi2MnP tetrahedra. In the thirty-first O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a distorted linear geometry to one V+4.67+ and one P5+ atom. In the thirty-third O2- site, O2- is bonded to two Li1+, one V+4.67+, and one P5+ atom to form distorted OLi2VP tetrahedra that share a cornercorner with one OLi2MnP tetrahedra and an edgeedge with one OLi2VP tetrahedra. In the thirty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.67+, and one P5+ atom. In the fortieth O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form distorted OLi2